Nowadays, adhesive industry is growing, and its development will be important in a short future because it offers good returns, and in some cases it is a better option for packaging and sealing with advantages in prices, productivity and weight reduction. In terms of joining and/or sealing, adhesives are well positioned among joining systems; however, knowledge about adhesives is need for their efficient use and only through proper design of the union can be achieved satisfactory results. In this chapter, a development of a formulation of pressure-sensitive adhesive based on styrene-butadiene copolymers using a reactive resin is reported. Non-aromatic solvents were used in adhesive formulation with the aim of avoiding the emission of harmful solvents into the Atmosphere, and the adequate combination and amount of solvents were found. The effect of addition of a phenolic resin in the adhesive formulation as a crosslinking agent was evaluated. By means Fourier Transform Infrared spectroscopy (FTIR), the crosslinking reaction was also studied. The performance of adhesive formulation was evaluated by means of dynamic mechanical analysis (DMA).
- reactive resin
- adhesive properties
- radial SBS
Adhesives have been used since ancient times, since the discovery of materials with adhesive properties from natural and animal resources. Then, through the study of the properties and appearance of new materials, several kinds of adhesives with synthetic components have been developed with the aim of improving their performance properties in specific application areas.
An adhesive is a material capable of joining two substrates through mechanisms of adhesion and cohesion through surface contact; it is applied over surfaces to keep them joined permanently. Also, the adhesives can be used as sealants.
Adhesion referred as the state between two bodies in intimal interfacial contact that transferred as interfacial forces in substrate area to carry out the joining or adhesion.
The adhesion phenomena can be understood by some theories: the adhesion chemical theory refers to intermolecular and Van Der Waals forces and chemical bonds that are generated between the adhesive and substrate. The diffusion theory explains the adhesion based on polymeric chain movements through the interphase, determining higher mobility according to molecular weight resulting in partial penetrations between materials. The weak limit layer theory proposes the existence of zones in the adhesion surface with cohesive breakages or weak joint forces originated by impurities in adhesive or adherent. The mechanical theory explains that adhesion can be achieved according to porosity and rugosity of the substrate surface when the adhesive penetrates forming anchor zones. The electrostatic theory proposes the formation of electrostatic forces at the adhesive-substrate interphase and is commonly applied in polymer-metal adhesion. The adsorption theory refers to the forces generated in the adhesive-substrate interface considering the superficial tension of adhesive to wetting the substrate and forming a contact angle .
The adhesive joint can be considered of two types: structural and non-structural. The structural adhesive joint is applied on substrates that experiment high deformations, over its yield point. This type of joints can be capable of transferring strain without loss in the integrity of the system in the design limits. The non-structural adhesive joints are those that do not require support substantial charges; its function is to keep materials of light weight in established place in the system of joint design. The sensitive adhesives to pressure and package adhesives are examples of non-structural adhesives.
1.1. Adhesive formulations
There are several types of adhesives that are developed in function of its final application, among contact adhesive base solvent with Polychloroprene for applications in wood, canvas and felt, etc. A disadvantage of these adhesives is when it comes to the environmental field, due to the kind of polymer, so it is necessary to find alternatives to replace Polychloroprene, styrene-butadiene-styrene copolymers (SBS) an option, using a reactive resin to obtain contact adhesive base solvent from equal or better performance. However, in attempts to establish a formulation with these components, there are some problems in stability and precipitation during storage; therefore, a formulation is required based on a proposal of resin and polymer that makes adhesives capable to cover all the performance parameters during storage and application.
On the other hand, development of adhesive formulations that are environmental friendly is a requirement according to several organizations, with the aim of covering regulations, because it is necessary for incorporation of substitution of harmful materials. Adhesives can be formulated by several paths, according to applications and compliance, which depends on cohesive and adhesive properties that can be tailored with a good polymer selection or amount of reactive resin or with the presence of another additive. Polychloroprene is one of the most used polymers in pressure-sensitive adhesive (PSA) formulations, because there are regulations that the material needs to be replaced. Among the materials that have been used in PSA formulations, styrene-butadiene copolymers represent a good option [2, 3]. In adhesive formulations, crosslinking reaction is the main step that controls the adhesive properties, and it can be carried out by means of addition of different agents; the most common crosslinking agent is sulphur , but organic peroxides and ester, ether and phenolic resins can also promote the crosslinking agent with appropriate conditions, for instance radiation, heat, change in pH, etc.
SP-154 is a heat-reactive phenolic resin that was developed for adhesive formulation; it is soluble in aromatic hydrocarbons and ketones and partially soluble in alcohols. Adhesive formulations with SP-154 resin have excellent heat resistance and high cohesive strength .
Styrene-butadiene copolymers (SBC) have a wide field of applications as shoe soles, impact modifiers, asphalt modifiers, adhesives and sealants. Several kinds of SBC have been used in adhesive formulations and as films in adhesives [2, 6, 7]; however, study of radial structure is not reported before.
There is a report that studied the adhesion properties of SBS copolymer and an epoxy resin after crosslinking with ultraviolet light, and that crosslinking grade of polybutadienic block was high and the adherence strength depends on the crosslinking level .
The amount and resin type in an adhesive formulation affect its performance, so it is necessary to evaluate the corresponding amounts to obtain the desired properties. Previous report  carried out the shear test for single overlap in cured probes using as substrate aluminium with adhesive formulations prepared with phenolic resin in different concentrations. According to the results, a higher resin concentration increases the shear strength; it was also found that the failure kind depends on resin concentration in formulation, so phenolic resin was shown to be an effective additive to improve adhesive properties.
An important characteristic to be considered in adhesive formulations is the polymer structure. Researchers prepared two copolymers, one of radial structure and the second one random from poly (methyl methacrylate) and poly (2-ethylhexylacrylate-co-methylacrylate), reporting high differences between block copolymer and random, due to the ability of the last one to form physical networks by phase separation .
1.2. Resin effect on adhesive
According to international standards ISO 472, ISO 4618/3, the resins are defined as “organic solids, semisolids or pseudo solids that have an indefinite and relative high molecular weight, and often melt over a wide temperature range”.
The resins have the following characteristics: average molecular weight lower than 10,000 g/mol, amorphous and complex structures, and do not exhibit a well-defined melt point, but have a glass transition temperature and softening temperature.
The resins can be divided into natural and synthetic. The first are from animal and vegetal sources; the second result from controlled chemical reactions and are divided into:
- Hydrocarbon resins that are produced by means of polymerization, and they are added to polymer to provide adhesion, flow and toughness.
- Synthetic resins obtained by addition polymerization and polycondensation; they are intermediates in plastic synthesis of high molecular weight .
The selection of resin for use in thermoplastic rubbers was based on its tendency to associate with intermediate or final block, depending on the desired effect on adhesive properties. The resin with softening point over 85°C tends to associate with the final copolymer blocks. This category of resins tends to provide rigidity to formulation and hold the cohesive strength in high temperature, and is used to improve the specific adhesion of the final block phase and adjust the flow viscosity .
1.3. Phenolic resins
The phenolic resins are used widely in industrial level due to its high thermal stability, toughness and stress resistance, and provide wide application areas especially in coatings, adhesives, insulation and laminates. The classic phenolic resins are resol and novalac; its structure can be modified to obtain desired properties in several applications .
The resol and novalac resins are intermediate reactive that under some transformations variety (for instance, novalac in production of poly (aril ether amides) and resol by means of reaction with acetals to produce wire varnish) among some improvements and in some cases improved resin systems that produce reactive resins for value-add products .
The phenolic resins are used also in combination with reinforcers such as carbon or fiberglass. In these systems, the mechanical properties are lower than when epoxy resin is used, but with better fire behaviour. One of the most important applications is in aircraft interiors.
The novalac resins are stable, thermoplastic, solid, soluble and meltable. They are prepared under acidic conditions with less than equimolar proportion of formaldehyde with phenol, and these kinds of resins are preferred to moulding materials . Figure 1 shows the obtaining of a contact adhesive using a resol resin.
In this kind of contact adhesives based on chloroprene (Figure 1) are added magnesium oxide and zinc, with the aim of acting as HCl acceptors and crosslinkers. The magnesium oxide plays an important role to form and no meltable but soluble metallic complex with phenolic resins. This complex improves the adhesive cohesive strength at high and room temperatures. The resins family of Terc-butylphenolics is the most widely used in neoprene adhesives because it provides high thermal resistance when reacting with magnesium oxide present in these formulations . The rubber properties change when crosslinked. These changes are reflected in thermoplasticity reduction, improving the abrasion and increasing tension strength.
1.4. Curing kinetic study
The chemical reactions involve formation and rupture of chemical bonding. The associate energy to a chemical bonding is a potential energy form, so that the chemical reactions involve potential energy changes. Often, for a reaction to occur, certain covalent bonds must be broken for others to emerge, which only occurs if the molecule orientation is appropriate to collide with enough kinetic energy to overcome the stabilization of potential energy of the bonds. The average kinetic energy of a molecule group is proportional to absolute temperature.
The kinetic contemplates the chemical reaction study and laws that govern that rate. The experimental fact that is based on the reaction rate of a system, at specific pressure and temperature, is only a state function. According to that, the basic equation of rate is:
Eq. (1) relates reaction rate
The activation energy
The frequency factor value of the collisions of
In the present work is reported the adhesive formulation based on a styrene-butadiene copolymer using a phenolic reactive resin. The effect of resin amount and combination of non-aromatic solvents was also studied. By means of infrared spectroscopy, the crosslinking reaction was monitored, and adhesive properties were evaluated by means of dynamic mechanical analysis and tensile test.
A thermoplastic copolymer styrene-butadiene-styrene (SBS) of radial block structure with polystyrene content of 30% and density of 0.94 g/cm3 provided by Dynasol Elastomers was used. As reactive resin, a commercial phenolic type resin named SP-154 from Ameripol Chemical S.A. de C.V. was used, with phenolic content >95%, formaldehyde content 200–400 ppm, melt point 79.4°C, flammability point 176.7°C and specific gravity 1.1 g/cm3; it was non-water soluble. As solvents were used ethyl acetate ≥99.5%, cyclohexane HPLC grade, Aldrich, and acetone ACS grade, Analytyka. The solvent selection was according to solubility parameter.
After proper solvent selection, solubility parameter of mix (
|Solvent||Solubility parameter||Phr||Volume fraction|
Adhesive formulation-based solvent consists of SBS elastomer, phenolic resin with commercial name SP-154, zinc oxide powder as filler and a mix of solvents (Table 2).
|Phenolic resin (SP-154)||0, 30, 50, 70|
|Zinc oxide||0, 1.0|
2.2. Adhesive preparation
Adhesive preparation consists of mixing all components in a Kettler glass reactor using a mechanical stirrer (IKA Euro-STPCV 600051 model) at 3500 rpm as maximum speed, at room temperature and 50% relative humidity. The material addition sequence was established according to several experimentations, based on solubility, dispersion, among others; first, SBS was added to solvent mix, after the zinc oxide and finally the phenolic resin and was continuously stirred for 2 h.
The thermogravimetric analysis (TGA) was carried out on materials in SDT2960 TA instrument equipment under a N2 atmosphere with 20 ml/min flow, in a temperature range from 40 to 600°C with 10°C/min rate, using 15 mg sample amount. DMA analysis was carried out in a DMA 2980 TA Instruments equipment, with a film tension clamp with multifrequency mode in a temperature range from −100 to 400°C with heat ramp of 5°C/min, 1 Hz of frequency and sample dimensions of 17 × 6 × 1 mm. Infrared (IR) analysis was carried out to evaluate crosslinking reaction and possible secondary reactions. IR spectra were recorded in Spectrum One Perkin Elmer equipment using the ATR technique with 12 scans and resolution of 4 cm−1 in wavenumber range of 4000–500 cm−1. Adhesive films were cured at 193°C, and different times since 0 until 60 min, with the aim of evaluating crosslinking process.
3. Results and discussion
3.1. Thermogravimetric analysis
From thermogravimetric analysis, with initial decomposition temperature, can be predicted the thermal stability of materials, and from the derivative curve of loss weight can be determined the maximum decomposition temperature.
Figure 2 shows the TGA thermogram where derivative indicates that region decomposition begins at 193°C, while at 217, 356 and 457°C other resin composites are degraded. Previous reports [17, 18] found a decomposition temperature at 199°C when a phenolic resin was used in adhesive formulation, mainly due to metylol and hydroxyl groups from phenolic structure. With higher phenolic group content, the temperature decomposition is lower. Around 350°C, this resin type can present active sites that condensed with metylol groups showing a constant degradation and at 400°C can be produced the breaking of phenolic groups with methyl groups from phenol structure.
3.2. Dynamic mechanical analysis (DMA)
DMA results were compared to evaluate the effect of resin in adhesive mixtures and the effect of addition of ZnO, monitoring the storage modulus and Tan
A non-uniform crosslinking has no considerable effect over the macroscopic properties of a material, such as
The transitions of adhesive formulations were determined by means of Tan
3.3. Kinetic study of crosslinking process
By means of DSC analysis, the curing parameters of adhesive formulations were determined, and the measurements were carried out in isothermal conditions at 180, 190, 200 and 210°C. From general reaction rate equation is possible to realize kinetic studies by following the reactions that were carried out in solid state in function of time at constant temperature according to the next equation :
By means of DSC, it was assumed that in material crosslinking during an exothermic process, the conversion rate is directly proportional to heat flow with the next equation :
For the crosslinking process to adjust to a model of order, the reaction kinetic is described as a function of conversion grade
It is assumed that reaction rate depends on the temperature; thus, the constant rate can be determined by means of the Arrhenius equation :
By means of lineal regression, the ln
The kinetic parameters
Using a multilinear regression, parameters
The adjust quality of dates from kinetic model can be noticed in graph ln
In Figure 5 are presented the isothermal curves obtained for adhesive formulation with 70 phr and zinc oxide at different temperatures, showing the influence of temperature in exothermic region, and Figure 6 shows the corresponding graph of calculating activation energy (ln
The selected temperature to obtain the kinetic parameters was 190°C, because it was closer to crosslinking reaction temperature. Table 3 shows the obtained kinetic values.
|Adhesive formulation||ln ||ln |
|Adhesive 0 phr||190||1.72||19.4||−3.8||98.07|
|Adhesive 30 phr resin||190||1.3||0.52||−4.77||24.91|
|Adhesive 50 phr resin||190||1.2||−1.44||−5.07||17.86|
|Adhesive 70 phr resin||190||1.28||−1.87||−5.27||15.38|
|Adhesive 0 resin phr ZnO||190||1.32||0.98||−4.14||61.98|
|Adhesive 30 phr resin ZnO||190||1.34||2.27||−4.61||33.46|
|Adhesive 50 phr resin ZnO||190||1.35||0.92||−4.77||26.85|
|Adhesive 70 phr resin ZnO||190||1.27||−1.24||−5.08||21.46|
From Table 3 the order reaction is 1 ≤
About the activation energy values from Table 3, it can be observed that resin content decreases the
The generous concentration of reactive sites and low viscosities in the initiation stage of crosslinking reaction contribute to increasing the degree of conversion after a time interval decelerates showing changes in the time reaction due the decreasing of availability of active sites and the increasing of viscosity, so the decreasing on reaction rate carry to the crosslinking reaction pass from chemical to diffusion control .
The physical properties of thermoplastics and elastomers used for crosslinking depend on the crosslinked structure, grade, time and crosslinking temperature; these parameters are related to network formation that provides substantial information about network structure and properties and processability .
3.4. FTIR characterization
FTIR technique was used to evaluate the crosslinking at different times (0, 20, 40 and 60 min, shorter times do not show significant effect), identifying the main functional groups that form or disappear when crosslinking reaction was carried out.
The crosslinking process is carried out by means of reaction of methylol and hydroxyl groups with unsaturations of polybutadiene . Initially, the decomposition reaction of resin by thermal effect generates active sites (methylol and hydroxyl) that stimulate the reaction to the formation of benzocarbenium ions with the double bond of the polybutadiene units to form cromane ring (Figure 7). Previous works [24, 25] prepare thermoplastic vulcanizate from natural rubber and high density polyethylene with and without compatibilizer, using an octyphenol formaldehyde resin using a compatibilizer obtaining good tensile strength and high elongation values, besides lower deformation compared with thermoplastic vulcanized without compatibilizer, which can be attributed to the formation of cromane ring of reaction. SBS copolymer and phenolic resin are present in an adhesive formulation.
Figure 8 shows the IR spectra for adhesive formulations with 30 phr resin without zinc oxide at different times. According to crosslinking reaction proposal, double bond of polybutadiene block has to decrease. The characteristic peak of C═C is at 1639 cm−1 and does not show a significant change with time; however, there is another peak attributed to ═C―H trans and ═CH2 vinyl at 963 and 910 cm−1, which present a decrease in intensity. The peaks from ═C―H cis at 727 cm−1 also show a decrease in intensity with time, which is indicative that crosslinking reaction of phenolic resin and SBS copolymer is carried out, mainly in cis structures. The polystyrene peaks at 1602 and 697 cm−1 do not show significant changes, which implies that crosslinking is not taking place in that polymer block. On the other hand, peaks attributed to phenolic resin are present at 3319, 1450, 1210 and 1026 cm−1, which present significative changes in intensity corroborating that crosslinking reaction is carried out with elastomer compared with elastomer without curing.
The peak at 1450 cm−1 corresponding to CH2 group increases due to the formation of methylene bonding between methylol groups of phenolic resin and some double bonds from polybutadiene block. At 1210 cm−1 peak attributed to C―O of phenols presents a decrease in intensity due to the influence of phenol in the crosslinking reaction. Figure 9 shows the IR spectra for adhesive formulations with zinc oxide. The changes in peaks are similar to those observed when zinc oxide is not added to adhesive formulation, which is indicative that it does not affect the crosslinking reaction. There are reports about the appearance of symmetric bands of OH groups that indicate breaking of hydrogen bonds and that over 200°C the OH group peak is indistinguishable [19, 26].
According to results, it is possible to obtain an adhesive formulation using solvents as an alternative for less environmental impact based on the solubility parameter that depends on the polymer used; in this case, solubility parameter found favours the polystyrene and polybutadiene blocks. The use of a reactive resin is an option to prepare adhesive formulations based on SBS elastomers. The inclusion of reactive resin affects the viscoelastic properties, due to the crosslinking process that was carried out as DMA results demonstrate; the best viscoelastic properties were observed for adhesive formulation with 30 phr of resin, and addition of zinc oxide was not favourable for adhesives. The results of kinetic study of crosslinking process indicate that addition of reactive resin is favourable for decreasing the
The present research work is registered in Tecnológico Nacional de México with code MAD-PYR-2015-0033. Two of the authors THM and MLMH thank CONACYT for the scholarship.
Packham DE, editor. Handbook of Adhesion. 2nd ed. Addison-Wesley Longman Ltd; 1992. 17 pp. 10.1002/0470014229
Salazar-Cruz BA, Mendoza-Martínez AM, Esquivel-de la Garza AC, Moctezuma Espíricueto SA, Rivera-Armenta JL. Evaluation of crosslinking reaction in adhesive based styrene-butadiene elastomers using infrared spectroscopy. In: Theophanides Theophile, editor. Infrared spectroscopy-anharmonicity of biomolecules, crosslinking ofbiopolymers, food quality and medical applications. InTech; 2015. p. 117-135. DOI 10.5772/58911.ch7.
Salazar-Cruz BA, Rivera-Armenta JL, García-Alamilla R, Mendoza-Martínez AM, Esquivel de la Garza A, Moctezuma Espiricueto S. Evaluación térmica del curado de adhesivos base SBR usando peróxido de dicumilo. Quimica Nova. 2015; 38:651-656. DOI 10.539/0100-4042.20150067.
Zielinska AJ. Cross-linking and Modification of Saturated Elastomers Using Functionalized Azides [Thesis]. Eindhoven, The Netherlands, University of Twente; 2011.
SI group, technical data sheet [Internet]. 2009. Available from: https://www.pharosproject.net/uploads/files/sources/1828/SP-154-1.pdf [Accessed: 2016-03-31].
Kim J, Kim WH, Lee DH. Adhesion properties of UV crosslinked polystyrene-block-polybutadiene block-polystyrene copolymer and tackifier mixture. Polymer. 2002; 43:5005-5010. DOI: 10.1016/S0032-3861(02)00327-0.
Navarro-Bañón MV, Pastor-Blas MM, Martín-Martínez JM. Elimination of the reactivation process in the adhesion of chlorinated SBS rubber with polychloroprene adhesives. eXPRESS Polymer Letters. 2007; 1:236-244. DOI: 10.3144/expresspolymlett.2007.36.
Sturiale A, Vazquez A, Cisilino A, Manfredi LB. Enhancement of the adhesive joint strength of the epoxy–amine system via the addition of a resole-type phenolic resin. International Journal of Adhesion and Adhesives. 2007; 156-164. DOI: 10.1016/j.ijadhadh.2006.01.007. 27:
Simal F, Jeusette M, Leclère PH, Lazzaroni R, Roose P. Adhesive properties of a radial acrylic block co-polymer with a rosin ester resin. Journal of Adhesion Science and Technology. 2007; 21:559-574. DOI:10.1163//156856107781192355.
Fink JK. Reactive Polymers Fundamentals and Applications: A Concise Guide to Industrial Polymers. 2nd ed. William Andrew. 2013. 29pp.
Skeist I, editor. Handbook of Adhesives. 3rd ed. International Thomson Publishing; 2011. 556 p.
Reghunadhan Nair CP, Bindu R L, Ninan KN. Thermal characteristics of addition-cure phenolic resins. Polymer Degradation and Stability. 2001; 73:251-257.DOI:10.1016/S0141-3910(01)00076-3.
Pilato L. Phenolic resins: 100 Years and still going strong. Reactive and Functional Polymers. 2013; 73:270-277. DOI:10.1016/j.reactfunctpolym.2012.07.008.
Scheneberger, G.L. editor. Adhesives in Manufacturing. 1st ed. Marcel Dekker. 1983. 353pp.
Tan D, Wang Y, Li Z, Xing H. Synthesis and cure kinetics of diphenyl (diphenylethynyl) silane monomer. Research on Chemical Intermediates. 2013; 39:3427-3440. DOI: 10.1007/s11164-012-0855-8.
Pérez JM, Oliet M, Alonso MV, Rodriguez F. Cure kinetics of lignin–novolac resins studied by isoconversional methods. Thermochimica Acta. 2009; 487:39-42. DOI: 10.1016/j.tca.2009.01.005.
Ginic-Markovic M, Choudhury NR, Dimopoulos M, Williams DR, Matisons J. Characterization of elastomer compounds by thermal analysis. Thermochimica Acta. 1998: 316:87-95. DOI: 10.1016/S0040-6031(98)00290-1.
Feng S, Yuan Z, Leitch M, Xu CC. Thermal degradation performance of bark based phenol formaldehyde adhesives. Journal of Analytical and Applied Pyrolysis. 2015; 115:184-193. DOI: 10.1016/j.jaap.2015.07.015.
Mangal R, Srivastava S, Archer LA. Phase stability and dynamics of entangled polymer-nanoparticle composites. Nature Communications. 2015: 6:1-9. DOI:10.1038/ncomms8198.
Rahul R, Kitey R. Effect of cross-linking on dynamic mechanical and fracture behavior of epoxy variants. Composites Part B: Engineering. 2016; 85,336-342. DOI: 10.1016/j.compositesb.2015.09.017.
Ren R, Xiong X, Ma X, Liu S, Wang J, Che P, Zeng Y. Isothermal curing kinetics and mechanism of DGEBA epoxy reins with phtalide-containing aromatic diamine. Thermochimica Acta. 2016; 623:15-21. DOI: 10.1016/j.tca.2015.11.011.
PerkinElmer Instruments LLC. Pyris Kinetics Software User Guide. 2002. Part Number 0996-6500, Release A.
Cai H, Li P, Sui G, Yu Y, Li G, Yang X, Ryu S. Curing kinetics study of epoxy resin/flexible amine toughness systems by dynamic and isothermal DSC. Thermochimica Acta. 2008; 473:101-105. DOI: 10.1016/j.tca.2008.04.012
Nakason C, Nuansomsri K, Kaesaman A, Kiatkamjornwong S. Dynamic vulcanization of natural rubber/high-density polyethylene blends: effect of compatibilization, blend ratio and curing system. Polymer Testing. 2006; 25:782-796. DOI: 10.1016/j.polymertesting.2006.05.001.
Scagliusi S, Cardoso E, Luga, A. Radiation-induced degradation of butyl rubber vulcanized by three different crosslinking systems. Radiation Physics and Chemistry. 2012; 81,991-994. DOI: 10.1016/j.radphyschem.2012.01.011.
Yue S, Juanfeng H, Hong H, Hequing F, Hanwei Z, Huanqin C. Synthesis, properties and application of a novel epoxidized soybean oil-toughened phenolic resin. Chinese Journal of Chemical Engineering. 2007; 15:418-423. DOI:10.1016/S1004-9541(07)60101-3.